determination of transmutation effects in crystalline waste forms /67531/metadc777063/...آ 3...
Post on 06-Jun-2020
Embed Size (px)
FINAL REPORT U. S. Department of Energy
Determination of Transmutation Effects in Crystalline Waste Forms
Principal Investigator: Jeffrey A. Fortner Argonne National Laboratory, Argonne, IL Collaborators: Donald T. Reed, A. Jeremy Kropf, and Rex E. Gerald Argonne National Laboratory, Argonne, IL Nancy J. Hess
Pacific Northwest National Laboratory, Richland, WA
Project Number: 55382 Grant Number: Grant Project Officers: Project Duration: October 1, 1996 to September 1, 1999
Table of Contents
Executive Summary 3
1 Research Objectives 7
2 Methods and Results 13
3 Relevance, Impact, and Technology Transfer 32
4 Project Productivity 33
5 Personnel Supported 34
6 Transfer 35
Publications Interactions Transitions Patents Future Work
7 Literature Cited 37
3 Transmutation Effects – Project 55382
The overall goal of this project was to study key scientific issues related to the long-term stability and performance of crystalline waste forms under consideration for containment and disposal of nuclear waste. Our research efforts were focused on development of techniques to study the effects of the radioactive decay of 137Cs to 137Ba in crystalline pollucite (CsAlSi2O6). Cesium-137 is a fission product of uranium and is a major contaminant at U.S. Department of Energy production facilities. Pollucite is an aluminosilicate (ceramic) waste form being considered for long-term storage of 137Cs.
If the structure of the pollucite is damaged by radioactive decay, it may be less effective at containing the 137Cs. Most work on radiation effects in waste forms has focused on structural damage from alpha radiation. However, beta radiation results in transmutation, which changes both the valence and the ionic radius of the element. The purpose of this project was to determine whether the chemical differences between cesium and barium reduce the structural integrity of the pollucite waste form. The techniques developed in these studies may also be useful for evaluating radiation damage in other crystalline waste forms.
The work focused on evaluation of several 137Cs sources originally fabricated for tumor treatment. These sources were small, sealed, stainless steel capsules containing pollucite in which varying amounts of the usual nonradioactive 133Cs had been replaced by radioactive 137Cs. The capsules ranged from 10 to 20 years old. It was expected that the decay of 137Cs to 137Ba would place the pollucite structure under significant strain, because previous studies showed that this structure can accommodate only about 10% Ba (by weight) of Ba, compared to 40% (by weight) of Cs. For comparison, we also studied nonradioactive pollucite and various other materials containing Cs and Ba.
To investigate the effects of transmutation on pollucite, we used three complementary analytical techniques: X-ray synchrotron studies (EXAFS/XANES), solid-state nuclear magnetic resonance (NMR), and transmission electron microscopy (TEM). The synchrotron and NMR approaches are highly developmental analytical approaches that push the envelope of existing capabilities.
This research was done as a collaboration between Argonne National Laboratory and Pacific Northwest National Laboratory.
4 Transmutation Effects – Project 55382
Synchrotron methods (XANES/EXAFS) were used to examine the Cs and Ba L-edge (at ~5-6 keV) and K-edge (~35-38 keV) x-ray absorption edges. These studies were done at the Advanced Photon Source at Argonne and at the Stanford Synchrotron Research Laboratory (SSRL) in Stanford, California. Subtle, yet significant, differences were noted between the K-edge spectra of the radioactive and nonradioactive samples. Powder x-ray diffraction (XRD) was also carried out at the SSRL. The interatomic distances determined by XRD and EXAFS are in agreement and show that the radioactive pollucite sample retains the expected tetragonal structure.
One of the oldest, most radioactive samples was chosen for TEM examination because it contained the most radiogenic barium—nearly 16% of the total cesium has decayed to barium—and was expected to show the largest effect.† The samples were examined at Argonne using a JEOL 2000 FX Mark II TEM operated at 200 keV accelerating energy. Bright field transmission images revealed a homogeneous, crystalline matrix, with no evidence of distinct barium phases or ex-solution phenomena resulting from the transmutation of 137Cs to 137Ba. Electron diffraction patterns were obtained from several portions of the sample. Excellent agreement between the observed diffraction spacings and literature values for pollucite indicates that no substantial damage was done to the crystal structure, despite substantial transmutation.
Solid-state NMR studies of nonradioactive pollucite containing milligram levels of Cs, Al, and Si were conducted at Argonne. The use of NMR to analyze solids is a recent extension of traditional solution-state NMR. Solid-state NMR can provide nearest neighbor information relevant to radionuclides within the crystalline waste form. Part of this effort was directed at the development of a miniature toroid cavity NMR detector suitable for handling a highly radioactive specimen. The most promising NMR results were obtained for 27Al at room temperature. These results indicate that this method may be able to distinguish the influence of Ba on Al, and thus on the tetragonal structure of pollucite, for example. Other results provided the first spectroscopic evidence that the pollucite framework differs for normal and Ba-containing pollucite. The NMR work was the most developmental of the three techniques used. We did not progress to NMR study of radioactive samples, but our success with nonradioactive samples will likely lead to applications beyond the
† Not all of the cesium in the samples is radioactive 137Cs. Thus, some Cs will remain after transmutation to barium is complete.
5 Transmutation Effects – Project 55382
pollucite samples studied. In particular, the success with aluminum is significant given the importance of Al in many waste forms under consideration.
We used several advanced techniques to assess structural effects caused by the beta-decay transmutation of 137Cs to 137Ba in radioactive pollucite that had aged for nearly one half- life of the 137Cs. This transmutation might affect the stability of the aluminosilicate pollucite crystal because of chemical differences between Cs+ and Ba2+. Although the amount of barium exceeded the amount the structure was expected to tolerate, our observations indicate that the pollucite structure remained remarkably unaffected by the transmutation. This suggests the presence of a metastable, yet robust, state. Although our observations are limited, these are, to our knowledge, the only available data in which transmutation effects have been isolated from other radiation damage phenomena. The virtual null result for transmutation effects on the pollucite is encouraging from a regulatory and modeling point of view. However, this behavior may not be characteristic of aged waste forms in general.
6 Transmutation Effects – Project 55382
1 Research Objectives
1.1 Purpose of Project
The overall goal of this Environmental Management Science Program project was to develop research tools to investigate the effect of transmutation, that is, the radioactive decay of a radioisotope to an isotope of another element, on the stability of a crystalline matrix. This process is an important issue in the assessment of the long-term stability, and hence performance, of a waste form. Most work on radiation effects in waste forms has focused on alpha radiation, which produces more displacements than beta radiation. However, beta radiation results in transmutation, which changes both the valence and the ionic radius of the element undergoing decay. These changes in coordination chemistry may destabilize the waste form and hence permit higher releases of the radionuclide contaminants to the accessible environment.
Little is known about the mobility of Cs in pollucite. Only a few studies [1-3] have examined leaching following transmutation or irradiation of pollucite or closely related aluminosilicates. These studies seem to have contradictory results. The results may indicate that prior to radiation- induced amorphization, the accumulated defects may lead to higher leachability of Cs , whereas once amorphization occurs, the Cs becomes trapped in the collapsed structure . A more thorough analysis of the effect of accumulated defects from both transmutation and ionization processes on the pollucite structure is needed to assess to the impact on Cs mobility.
In this three-year research program, we used cutting-edge experimental approaches to investigate this little-understood issue. The work was a collaboration between Argonne National Laboratory (ANL) and Pacific Northwest National Laboratory (PNNL). We focused on the effects of transmutation on pollucite (CsAlSi2O6), a cesium aluminosilicate that has been proposed for the long-term immobilization of radioactive cesium. In this ceramic waste form, the 137Cs decays to 137Ba, causing barium to build up in the pollucite samples over time. We selected pollucite for this study for the following re